
Research Article


Stress Analysis on Direct Joining of Sialon to AISI 430 Ferritic Stainless Steel


C.S. Hassan,
P. Hussain
and
M. Awang



ABSTRACT

Finite Element Method (FEM) using ANSYS software was employed to evaluate the residual stress distribution in direct joining of sialon and AISI 430 ferritic stainless steel. The elasticplastic model and four nodes quadratic element PLANE 42 with axisymmetric option were adopted in the analysis. Results showed that sialon experience compressive stresses in radial direction but tensile in axial direction. On the other hand, stresses in AISI 430 ferritic stainless steel are tensile in radial direction but compressive in axial direction. The highest tensile axial stress appeared at the radial free surface of sialon, very near to the joint interface. It is observed that shear stresses concentrated near and on the joint interface.





Received:
October 22, 2010; Accepted: November 01, 2010;
Published: April 18, 2011 

INTRODUCTION
Ceramic has been the material of choice for high temperature applications such
as in internal combustion engine. In its application, ceramics are often in
contact with metal. For example, in ceramic turbocharger rotors, each ceramic
rotor requires attachment to a metal shaft, as illustrated by one of the rotors
in Fig. 1 (Richerson, 2006). Ceramic/metal
joint will take the advantage of metal toughness and the ability of ceramic
to withstand high temperature. Furthermore, the brittleness of ceramic can also
be overcome through this joining. However, successful ceramic/metal joints are
difficult to obtain due to the rise of residual stresses in the joint.
 Fig. 1: 
Example of ceramic turbocharger rotors, one illustrating
attachment to a metal shaft (Richerson, 2006) 
Residual stresses result from mismatches in the coefficient of thermal expansion
and elastic modulus of the base materials. Upon cooling from the relatively
high joining temperatures, characteristics of usual joining processes, the interface
restricts the contraction of the material, concentrating local stresses (Martinelli,
1996). Such stresses can cause plastic deformation and cracking and thereby
affect the mechanical integrity of the bonded materials (Lee
and Kim, 1997).
Figure 2 shows the typical fracture mechanism that occurs
in ceramic metal joint. When the joint is strong enough, mode I crack initiation
occurs in the ceramic at this point. The stress becomes compressive soon after
but maximum shear stress values are observed. As a consequence, mode I rapidly
transforms to mode II crack propagation in the ceramic close and along the joint
(Moret and Eustathopoulos, 1993; Lu
and Evans, 1985). Mechanical attachments invariably result in residual stress
concentration which may initiate cracks and cause failure (Hattali
et al., 2009a). It must be pointed out that tensile stresses in the
ceramic substrate, experimentally observed by Xray diffraction, are harmful
for the joint integrity since ceramic materials cannot withstand high tensile
stress (Vila et al., 2005; Zhihong
et al., 2009). Therefore, it is essential to evaluate the residual
stress state in the joint.
An effective approach to predict and analyze the magnitude and distribution of the residual stresses along a joint based on the particular properties of the materials to be joined is the Finite Element s Method (FEM).  Fig. 2: 
Typical fracture mechanism of a ceramic/metal assembly. If
the joint is strong enough, mode I crack initiation occurs on the lateral
surface of the ceramic in the maximum tensile stress area and mode II crack
propagation follows in the ceramic along the joint in the maximum shear
stress area 
 Fig. 3: 
Countermap of maximum principal stress calculated by FEM.
The joint is assumed to be cooled from 1073K to room temperature fully elastically.
The arrows indicate the position and direction of the maximum tensile stress
(Suganuma et al., 1985) 
Extensive studies had been carried out to study the residual stresses of ceramicmetal
joints using FEM. According to, Travessa et al. (2002),
once the bonding is obtained, the strength of the joint is primarily dependent
on the residual stresses at the interface. These stresses, originated from the
thermal expansion mismatch between the metallic and the ceramic substrates and
constructed during the cooling down from the bonding temperature, were first
quantified by analytical method (Virkar et al., 1987).
Later, FEM began to be applied not only to quantify residual stresses, but
also to describe the stress field. Suganuma et al.
(1985) had shown that maximum tensile stress concentrates on or near the
interface and the free surface, as presented in Fig. 3. Xiaoqin
et al. (2008) had calculated the residual stress distribution in
Al_{2}O_{3}–TiC/W18Cr4V diffusion bonded joints using FEM.
Vila et al. (2007) had used FEM calculations
to simulate the joining process and residual strains of cubeshaped Ni/Si_{3}N_{4
}specimens. Williamson et al. (1995) had
used FEM to study the effects of interlayer and creep in reducing residual stresses
and strains in ceramic to metal joints. Several research works, such as by Drake
et al. (1993) had used finite element numerical models and diffraction
measurements to investigate residual stresses developed at bonded Al_{2}O_{3}Ni
interfaces. Raevska (1998) had also used FEM to study
the dependence of residual stresses developed in ceramic metal joint on some
design and technology parameters. Suganuma et al.
(1984) by finite element analytical model, had showed that in joining dissimilar
materials, there is formation of axial tensile stresses near the free surfaces
of the materials with lower thermal expansion coefficient, adjacent to the interface,
during cooling.
The key to successful numerical analyses relies on the selection of materials
property, the proposed mechanisms for interface formation, and the development
of elastic or elasticplastic deformation models (Martinelli,
1996). The accuracy of FEM results further improved as elastoplastic behavior
of the metallic component started to be adopted in the model (Williamson
et al., 1995).
MATERIALS AND METHODS
The aim of the present work is to numerically evaluate the magnitude and distribution
of residual stresses in sialon/AISI 430 Ferritic Stainless Steel (FSS) joint
by means of Finite Element Analysis (FEA). Sialon was chosen as they present
excellent mechanical properties at high temperature. However, they cannot in
general be use alone due to their brittleness. On the other hand, stainless
steel is tough but operates at low temperature. Therefore, it is preferable
to join them in order to utilize the strength of both materials.
 Fig. 4: 
Model description, (a) schematic representation of the model
geometry resulted from the geometric simplification, showing the dimensions
used in the analysis and (b) details on meshing and constrains employed 
Table 1: 
Material properties of sialon and AISI 430 FSS employed in
the analysis 

FEA was applied to determine the magnitude and distribution of the residual stress in the sialon/AISI 430 FSS joint. The analysis was carried out using ANSYS 11 provided in the CAE/CFD lab of Universiti Teknologi PETRONAS. A cylindrical shaped AISI 430 FSS of 14 mm in diameter and 15 mm in thickness with 15 mm thickness of sialon on the top surface was considered. Sialon was treated as elastic while plasticity permitted within AISI 430 FSS. Elastoplastic regime for the metal which governed by von Mises yield and isotropic hardening were adopted. Material response is assumed to be independent of time. Coefficient of thermal expansion (CTE), modulus of elasticity, poison’s ratio as well as fracture and yield stress for sialon and AISI 430 FSS are given in Table 1. Only thermal loading was employed to the model as sialon and stainless steel are assumed to be perfectly bonded at the interface at the fabrication temperature of 1200°C and stresses only developed during cooling down to room temperature. Since the model geometry is symmetrical in axial direction, the problem was analyzed as twodimensional problem, as in Fig. 4. The fournode quadrilateral element PLANE42 with axisymmetric option has been used to model the joint. The model was imparted with mapped meshing with decreased element size as approaching the interface and free surface of the joint. The left boundary of the mesh corresponds to the symmetry axes were constrained in radial direction. All other boundaries remain free as to permit bending to occur during cooling. Details of meshing and constrains employed are in Fig. 4b. RESULTS AND DISCUSSION
Figure 5 shows the distributions of radial, σ_{x},
axial, σ_{y,} and shear stresses, τ_{xy,} across the
joint. With regards to specimen failure during cooling, the large tensile stresses
within the ceramic near the radial free surface appear to be the most significant
(Suganuma, 1990). This observation is consistent with
the radial stresses distribution obtained by FEM, as in Fig. 5b.
Do Nascimento et al. (2003) had stated that concentration
of residual stress becomes severer as closing to the interface. The pattern
of shear stresses distribution for sialon/ AISI 430 FSS joint agrees reasonably
well with the statement. It can be seen in Fig. 5c that the
shear stresses distribution concentrated on and near the interface of the joint.
These stresses, in combination with the maximum axial tensile stress located
at the free radial surface of sialon, clearly depicted the typical “concave/convex”
fracture that sometimes observed in a joint with large thermal expansion mismatch
(Do Nascimento et al., 2003).
 Fig. 5: 
Contour plots of the thermal residual stress distribution
for the sialon/AISI 430 FSS joint: (a) radial stress (σ_{x});
(b) axial stress (σ) and (c) shear stress (τ_{x}) 
In order to further analyze the magnitude and stress distribution across the joint, the stresses were plotted against the thickness of the seal. Radial stresses along the symmetry axes were plotted against thickness of the seal. Meanwhile, since axial and shear stresses rise to peak value at the radial free surface, stresses along the radial free surface were plotted against thickness of the seal. The plots of stresses magnitude against thickness are mentioned in Fig. 6. Thickness represented in Fig. 6 is measure from the bottom of the joint modeled. Thickness of AISI 430 FSS start from 0 up to the joint interface of 15 mm and thickness of sialon started right after the joint interface.
Figure 6a shows that, at the region near to the interface
of the joint where thickness equal to 1.5 mm, high tensile stress developed
in steel while ceramic experienced very low compressive stress. This is due
to thermal expansion mismatch of AISI 430 FSS and sialon. AISI 430 FSS with
higher CTE contracted more during cooling of the joint from the joining temperature.
However, its contraction was restrained by its bonding to sialon, thus resulting
in compressive stresses on the ceramic side. AISI 430 FSS reacted to that tendency,
trying to extend the interface, yielding the concentration of tensile stresses,
especially near the interface (Hattali et al., 2009a).
The maximum radial tensile stress in the AISI 430 FSS is equal to 367.23 MPa
while the minimum compressive stress in sialon is equal to 251.14 MPa. The stresses
stabilize to nearly zero stresses when the distance is further away from the
interface.
Figure 6b shows that axial stresses, represented as S_Y in
ANSYS, are tensile in sialon while compressive in steel. The compressive stresses
developed in AISI 430 FSS might be due to the effect of yielding of the steel
(Cao et al., 1988). The maximum axial stress
is about 509.53 MPa located on the free surface of sialon, around 0.23 mm from
the joint interface. This is belief to be the crack initiation point if any
fracture occurs in the sialon/AISI 430 FSS joint. Cao et
al. (1988) had stated that ceramic parts near the interface have high
tensile residual stress and are prone to cracking. The cracks initiated at the
edge will downgrade the ceramic properties and may even lead to fracture.
 Fig. 6: 
Stress magnitude across sialon/ AISI 430 FSS joint, (a) radial
stresses along the axis symmetry, and (b) axial and shear stresses along
the radial free surface of the joint 
It can be seen that the amplitude of σ_{y} decreases as the distance
from the interface decreases. On the sialon side, σ_{y} tensile
stresses decreases and starts to stabilize to a nearly zero stresses at a distance
of 1.1 mm away from the joint interface. Meanwhile, on the AISI 430 FSS side,
σ_{y} is compressive in nature. The axial residual stresses decrease
and achieved nearly zero magnitude of stress at a distance of 1.2 mm from the
interface. The decreases of compressive σ_{y } in AISI 430 FSS
might be as a result of the plastic deformation of the metal (Hattali
et al., 2009b).
As can be seen in Fig. 6b, the tensile shear stresses, represented
as S_XY in ANSYS, start developed in steel around 1.5 mm from the interface,
and the stresses remain tensile in the ceramic up to around 1.5 mm from the
interface. Maximum tensile shear stress of 106.69 Mpa developed at the sialon/
AISI 430 FSS joint interface. Also, it can be observed that on both sialon and
AISI 430 FSS sides, like axial stresses, the amplitude of shear stresses also
increase rapidly as approaching the joint interface and decreases to nearly
zero stresses as moving further away from the interface.
Thermal expansion coefficient mismatch effect is a serious problem because,
even if a strong interface could be achieved, joints with large residual stress
are easily broken (Suganuma et al., 1987). The
developments of residual stresses originated from the thermal expansion mismatch
and induced during cooling down from the fabrication temperature strongly influence
the joint integrity. Materials with low elastic modulus can accommodate strain
and tend to deform under the influence of these stress. However, brittle material
such as ceramic and glass will have a tendency to fracture. Sialon, like any
other ceramic can bear with compressive stress but not tensile stress. They
tend to fracture under the influence of high tensile stress. After evaluating
all the stresses developed in the sialon/ AISI 430 FSS joint, it can be seen
that the highest stress induced is the axial stress located in the free surface
of the ceramic. In the case of sialon/ AISI 430 FSS joint with dimensions and
fabrication temperature as described above, maximum axial tensile stress that
developed in the sialon is equal to 509.53 Mpa. Even though the stress is considerably
high, but the stress still did not exceed the ceramics’ fracture stress
of 825 MPa. This brings the possibility of successful direct joining of sialon
to AISI 430 FSS.
CONCLUSION The residual stresses generated in sialon/ AISI 430 FSS joint during cooling down from the fabrication temperature were predicted by the numerical model proposed. It was found that sialon experienced compressive stresses in axial direction but tensile in radial direction. On the other hand, AISI 430 FSS experienced tensile stress in radial direction but compressive in axial direction. Maximum tensile stress located on free radial surface of sialon, very near to the joint interface. It was also observed that shear stresses distribution concentrated on and near the interface of the joint. Since the maximum tensile stress developed in sialon did not exceed the fracture stress of the ceramic, it can be said that the joint is successful. Under specific conditions, joints can be obtained between sialon and AISI 430 FSS by means of bonding at the fabrication temperature of 1200°C. The magnitude and distribution of all stresses are stabilized to a very low stress as moving further away from the interface. FEM had resulted in a very satisfactory description on magnitude and distribution of stresses in the ceramic/metal joint. Therefore numerical simulation can be used for assessing residual stress in ceramic/metal joint and as a guide in component fabrication. This method can be used as an alternative for trial and error experimental work as it is more time saving and reducing material consumption. However, further experimental work is still recommended as to provide evidence for the FEM calculation. ACKNOWLEDGEMENT This research was made possible by a grant and facilities provided by Universiti Teknologi PETRONAS.

REFERENCES 
Cao, H.C., M.D. Thouless and A.G. Evans, 1988. Residual stresses and cracking in brittle solids bonded with a thin ductile layer. Acta Metall., 36: 20372046. CrossRef 
Do Nascimento, R.M., A.E. Martinelli and A.J.A. Buschinelli, 2003. Review article: Recent advances in metalceramic brazing. Ceramica, 49: 178179.
Drake, J.T., R.L. Williamson and B.H. Rabin, 1993. Finite element analysis of thermal residual stresses at graded ceramic/metal interfaces, part II: Optimization for residual stress reduction. J. Applied Phys., 74: 13211326. CrossRef 
Hattali, M.L., S. Terekhina, F. Ropital, N. Mesrati and D. Treheux, 2009. Optimization of fabrication parameters of Alumina/Nickel alloy joints for hightemperature application. IOP Conf. Ser. Mater. Sci. Eng., 5: 012011012011. CrossRef 
Hattali, M.L., S. Valette, F. Ropital, N. Mesrati and D. Treheux, 2009. Effect of thermal residual stresses on the strength for both alumina/Ni/alumina and alumina/Ni/nickel alloy biomaterials. J. Mater. Sci., 44: 31983200. CrossRef 
Lee, S.B. and J.H. Kim, 1997. Finiteelement analysis and Xray measurement of the residual stresses of ceramic/metal joints. J. Mater. Process. Technol., 67: 167172. CrossRef 
Lu, M.C. and A.G. Evans, 1985. Influence of cyclic tangential loads on indentation fracture. J. Am. Ceramic Soc., 68: 505510. CrossRef 
Martinelli, A.E., 1996. Diffusion bonding of silicon carbide and silicon nitride to molybdenum. Ph.D. Thesis, McGill University, Canada.
Moret, F. and N. Eustathopoulos, 1993. Ceramic to metal direct brazing. J. Phys. IV, 3: C71043C71052. CrossRef 
Raevska, S., 1998. Reduction of the stresses introduced during the diffusion bonding of dissimilar materials. J. Mater. Process. Technol., 77: 5053. CrossRef 
Richerson, D.W., 2006. Modern Ceramic Engineering: Properties, Processing and Use in Design. 3rd Edn., Taylor and Francis Group, London.
Suganuma, K., 1990. Review: Recent advances in joining technology of ceramics to metals. ISU Int., 30: 10461058.
Suganuma, K., T. Okamoto and M. Koizumi, 1984. Effect of interlayers in ceramicmetal joints with thermal expansion mismatches. J. Am. Ceramic Soc., 67: C256C257. CrossRef 
Suganuma, K., T. Okamoto, M. Koizumi and K. Kamachi, 1987. Influence of shape and size on residual stress in ceramic/metal joining. J. Mater. Sci., 22: 35613565. CrossRef 
Suganuma, K., T. Okamoto, M. Koizumi and M. Shimada, 1985. Effect of thickness on direct bonding of silicon nitride to steel. J. Am. Ceramic Soc., 68: 334335. CrossRef 
Travessa, D., M. Ferrante and G. den Ouden, 2002. Diffusion bonding of aluminum oxide to stainless steel using stress relief interlayers. Mater. Sci. Eng. A, 337: 287296. CrossRef 
Vila, M., C. Prieto, J. Zahr, J.L. PerezCastellanos and G. Bruno et al., 2007. Residual stresses in ceramictometal joints: Diffraction measurements and finite element method analysis. Philosophical Mag., 87: 55515563. CrossRef 
Vila, M., C. Prieto, P. Miranzo, M.I. Osendi, J.M. Del Rio and J.L. PerezCastellanos, 2005. Measurements and finiteelement simulations of residual stress developed in Si3N4/Ni diffusion bonds. J. Am. Ceram. Soc., 88: 25152520. CrossRef 
Virkar, A.V., J.L. Huang and R.A. Cutler, 1987. Strengthening of oxide ceramics by transformationinduced stress. J. Am. Ceramic Soc., 70: 164170. CrossRef 
Williamson, R.L., B.H. Rabin and G.E. Byerly, 1995. FEM study on the effects of interlayers and creep in reducing residual stresses and strains in ceramicmetal joints. Composite Eng., 5: 851863. CrossRef 
Xiaoqin, S., L. Yajiang, U.A. Putchkov, J. Wang and W. Huang, 2008. Finiteelement analysis of residual stresses in Al_{2}O_{3}TiC/W18Cr4V diffusion bonded joints. Comput. Mater. Sci., 45: 407410. CrossRef 
Zhihong, Z., Z. Zhangjian and G. Changchun, 2009. Brazing of doped graphite to Cu using stress relief interlayers. J. Mater. Process. Technol., 209: 26622670. CrossRef 



